#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:56:04 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180523 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/92/7219299.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7219299
loop_
_publ_author_name
'Jiao, Yan-Qing'
'Qin, Chao'
'Zang, Hong-Ying'
'Chen, Wei-Chao'
'Wang, Chun-Gang'
'Zheng, Tian-Tian'
'Shao, Kui-Zhan'
'Su, Zhong-Min'
_publ_section_title
;
 Assembly of organic--inorganic hybrid materials constructed from
 polyoxometalate and metal--1,2,4-triazole units: synthesis, structures,
 magnetic, electrochemical and photocatalytic properties
;
_journal_issue                   10
_journal_name_full               CrystEngComm
_journal_page_first              2176
_journal_paper_doi               10.1039/C4CE02007C
_journal_volume                  17
_journal_year                    2015
_chemical_formula_moiety         'C16 H50 Cl2 Cu6 N24 O55 Si W12'
_chemical_formula_sum            'C16 H50 Cl2 Cu6 N24 O55 Si W12'
_chemical_formula_weight         4145.23
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_block_doi                 10.5517/cc13895v
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;
_cell_angle_alpha                94.051(5)
_cell_angle_beta                 105.611(5)
_cell_angle_gamma                105.770(5)
_cell_formula_units_Z            1
_cell_length_a                   11.5350(5)
_cell_length_b                   12.0910(5)
_cell_length_c                   14.3130(5)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.000
_cell_measurement_theta_min      1.800
_cell_volume                     1827.83(15)
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0371
_diffrn_reflns_av_unetI/netI     0.0694
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            10539
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        24.997
_diffrn_reflns_theta_max         24.997
_diffrn_reflns_theta_min         1.771
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    20.703
_exptl_absorpt_correction_T_max  0.035
_exptl_absorpt_correction_T_min  0.032
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_crystal_colour            'dark green'
_exptl_crystal_density_diffrn    3.766
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1864
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.16
_platon_squeeze_details
;
;
_refine_diff_density_max         2.946
_refine_diff_density_min         -5.367
_refine_diff_density_rms         0.443
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     505
_refine_ls_number_reflns         6404
_refine_ls_number_restraints     730
_refine_ls_restrained_S_all      1.019
_refine_ls_R_factor_all          0.0904
_refine_ls_R_factor_gt           0.0688
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0887P)²+94.5388P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1701
_refine_ls_wR_factor_ref         0.1862
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4948
_reflns_number_total             6404
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c4ce02007c2.cif
_cod_data_source_block           4
_cod_depositor_comments
'Adding full bibliography for 7219296--7219301.cif.'
_cod_original_cell_volume        1827.83(14)
_cod_database_code               7219299
#BEGIN Tags that were not found in dictionaries:
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
#END Tags that were not found in dictionaries
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
O1 O -0.0184(16) 0.2243(15) 0.3404(14) 0.046(2) Uani 1 1 d . U .
O2 O 0.2173(16) 0.2322(15) 0.4173(13) 0.043(2) Uani 1 1 d . U .
O3 O 0.1402(13) 0.0798(12) 0.5813(10) 0.0227(7) Uani 1 1 d . U .
O4A O 0.301(3) 0.135(3) 0.549(3) 0.038(2) Uani 0.5 1 d . U P
O4B O 0.370(3) 0.179(3) 0.594(3) 0.037(2) Uani 0.5 1 d . U P
O5 O 0.2626(17) 0.0516(15) 0.7109(14) 0.046(2) Uani 1 1 d . U .
O6 O 0.4686(18) 0.0168(16) 0.6566(16) 0.055(4) Uani 1 1 d . U .
O7 O 0.2295(17) -0.1472(16) 0.6171(14) 0.051(2) Uani 1 1 d . U .
O8 O 0.1007(15) -0.0730(14) 0.4986(12) 0.0344(13) Uani 1 1 d . U .
O9 O 0.2911(18) -0.0394(16) 0.4700(16) 0.0564(18) Uani 1 1 d . U .
O10 O 0.1047(18) -0.2456(17) 0.4297(15) 0.055(3) Uani 1 1 d . U .
O11 O 0.2348(19) -0.1750(16) 0.2942(16) 0.058(4) Uani 1 1 d . U .
O12 O 0.0204(15) -0.0169(13) 0.3952(12) 0.0315(10) Uani 1 1 d . U .
O15 O 0.0478(14) 0.1240(12) 0.4643(11) 0.0256(7) Uani 1 1 d . U .
O16 O 0.0984(16) 0.3218(15) 0.5273(13) 0.041(2) Uani 1 1 d . U .
O17 O 0.3619(15) 0.3913(14) 0.5832(12) 0.035(2) Uani 1 1 d . U .
O18 O -0.108(2) 0.3836(15) 0.4241(15) 0.054(4) Uani 1 1 d . U .
O19 O 0.1278(19) 0.2081(19) 0.2223(16) 0.063(5) Uani 1 1 d . U .
O20 O 0.1746(17) 0.0289(15) 0.3169(14) 0.047(2) Uani 1 1 d . U .
O21A O 0.192(3) 0.232(3) 0.660(3) 0.036(2) Uani 0.5 1 d . U P
O21B O 0.249(3) 0.271(3) 0.704(3) 0.033(3) Uani 0.5 1 d . U P
O22 O 0.2337(19) 0.1840(17) 0.8638(14) 0.057(4) Uani 1 1 d . U .
O23 O 0.0641(17) -0.0260(15) 0.7629(14) 0.046(3) Uani 1 1 d . U .
O24 O -0.0070(17) -0.1729(16) 0.2780(15) 0.051(3) Uani 1 1 d . U .
Si1 Si 0.0000 0.0000 0.5000 0.0280(13) Uani 1 2 d S U P
Cu1 Cu 0.5000 0.5000 0.5000 0.0187(7) Uani 1 2 d S . P
Cu2 Cu 0.5310(2) 0.5122(3) 0.76132(19) 0.0263(6) Uani 1 1 d . . .
Cu3 Cu 0.5000 0.5000 1.0000 0.0316(9) Uani 1 2 d S . P
W1 W 0.15632(11) 0.12538(9) 0.74777(7) 0.0399(3) Uani 1 1 d . U .
W2 W 0.31421(9) 0.00704(10) 0.60525(10) 0.0463(3) Uani 1 1 d . U .
W3 W 0.15818(9) -0.12084(9) 0.35890(8) 0.0361(3) Uani 1 1 d . U .
W4 W 0.24191(9) 0.26557(7) 0.55830(8) 0.0338(3) Uani 1 1 d . U .
W5 W 0.08776(9) 0.13962(8) 0.31011(7) 0.0306(3) Uani 1 1 d . U .
W6 W -0.07232(9) 0.26029(7) 0.44999(8) 0.0319(3) Uani 1 1 d . U .
N1 N 0.5299(16) 0.3703(16) 0.9230(13) 0.026(4) Uani 1 1 d . U .
N2 N 0.5384(17) 0.3696(18) 0.8291(13) 0.032(5) Uani 1 1 d . . .
N3 N 0.6557(17) 0.4885(18) 0.7012(13) 0.031(4) Uani 1 1 d . . .
N4 N 0.6476(15) 0.4849(14) 0.6015(11) 0.018(3) Uani 1 1 d . U .
N5 N 0.5230(18) 0.6445(17) 0.6849(14) 0.031(4) Uani 1 1 d . . .
N6 N 0.5026(15) 0.6397(16) 0.5860(11) 0.021(4) Uani 1 1 d . . .
N7 N 0.531(2) 0.819(2) 0.6452(18) 0.052(6) Uani 1 1 d . U .
H10 H 0.5418 0.8927 0.6506 0.063 Uiso 1 1 calc R U .
N9 N 0.559(2) 0.2090(19) 0.8736(16) 0.045(5) Uani 1 1 d . U .
H9 H 0.5702 0.1413 0.8739 0.053 Uiso 1 1 calc R U .
N10 N 0.8390(15) 0.4834(16) 0.6833(13) 0.024(4) Uani 1 1 d . . .
Cl1 Cl 0.6683(6) 0.6439(6) 0.9217(4) 0.0471(16) Uani 1 1 d . . .
C1 C 0.559(3) 0.275(3) 0.802(2) 0.058(8) Uani 1 1 d . . .
H1 H 0.5711 0.2556 0.7424 0.070 Uiso 1 1 calc R U .
C2 C 0.7590(19) 0.4795(19) 0.5940(15) 0.024(5) Uani 1 1 d . . .
H2 H 0.7787 0.4739 0.5354 0.029 Uiso 1 1 calc R U .
C3 C 0.773(2) 0.492(2) 0.7466(17) 0.029(5) Uani 1 1 d . U .
H3 H 0.8063 0.5001 0.8144 0.035 Uiso 1 1 calc R U .
C4 C 0.532(3) 0.751(2) 0.718(2) 0.054(7) Uani 1 1 d . U .
H4 H 0.5385 0.7767 0.7820 0.064 Uiso 1 1 calc R U .
C5 C 0.509(2) 0.7472(19) 0.567(2) 0.040(6) Uani 1 1 d . . .
H5 H 0.4986 0.7680 0.5049 0.048 Uiso 1 1 calc R U .
C6 C 0.540(3) 0.271(3) 0.942(2) 0.056(8) Uani 1 1 d . . .
H6 H 0.5344 0.2456 1.0007 0.067 Uiso 1 1 calc R U .
Cu4 Cu 1.0103(2) 0.4904(3) 0.7254(2) 0.0379(7) Uani 1 1 d . . .
N8 N 1.1792(16) 0.5003(18) 0.7800(13) 0.032(5) Uani 1 1 d . . .
C7 C 1.270(2) 0.516(2) 0.7365(17) 0.030(5) Uani 1 1 d . U .
H7 H 1.2569 0.5255 0.6710 0.037 Uiso 1 1 calc R U .
C8 C 1.242(2) 0.491(2) 0.8736(17) 0.033(5) Uani 1 1 d . U .
H8 H 1.2042 0.4799 0.9237 0.040 Uiso 1 1 calc R U .
O1W O 0.538(4) -0.019(3) 0.895(3) 0.140(10) Uani 1 1 d . U .
N11 N 1.3759(16) 0.5168(15) 0.7932(12) 0.023(4) Uani 1 1 d . U .
N12 N 1.3605(18) 0.501(2) 0.8840(14) 0.037(5) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
W6 O1 W5 137.3(11) . .
W5 O2 W4 135.4(10) . .
Si1 O3 W4 120.4(7) . .
Si1 O3 W1 120.3(6) . .
W4 O3 W1 97.6(5) . .
Si1 O3 W2 118.8(7) . .
W4 O3 W2 97.1(5) . .
W1 O3 W2 97.5(5) . .
O4B O4A W2 91(3) . .
O4B O4A W4 85(3) . .
W2 O4A W4 142(2) . .
O4A O4B W4 69(3) . .
O4A O4B W2 64(3) . .
W4 O4B W2 120.4(17) . .
W1 O5 W2 143.9(11) . .
W2 O7 W6 136.1(11) . 2_556
Si1 O8 O12 54.6(7) . .
Si1 O8 W3 124.1(9) . .
O12 O8 W3 69.5(7) . .
Si1 O8 W6 121.4(8) . 2_556
O12 O8 W6 134.9(10) . 2_556
W3 O8 W6 96.3(6) . 2_556
Si1 O8 W2 118.6(8) . .
O12 O8 W2 128.5(9) . .
W3 O8 W2 95.2(5) . .
W6 O8 W2 94.3(6) 2_556 .
W3 O9 W2 137.5(11) . .
W6 O10 W3 137.1(12) 2_556 .
Si1 O12 O8 57.5(7) . .
Si1 O12 O15 56.5(7) . .
O8 O12 O15 94.8(10) . .
Si1 O12 W5 124.0(8) . .
O8 O12 W5 133.4(10) . .
O15 O12 W5 67.5(6) . .
Si1 O12 W3 123.5(8) . .
O8 O12 W3 66.0(7) . .
O15 O12 W3 133.6(9) . .
W5 O12 W3 94.7(5) . .
Si1 O12 W1 120.4(8) . 2_556
O8 O12 W1 127.9(9) . 2_556
O15 O12 W1 129.0(9) . 2_556
W5 O12 W1 93.2(5) . 2_556
W3 O12 W1 92.9(5) . 2_556
Si1 O15 O12 54.7(6) . .
Si1 O15 W5 122.6(8) . .
O12 O15 W5 67.8(6) . .
Si1 O15 W4 120.6(8) . .
O12 O15 W4 129.9(9) . .
W5 O15 W4 95.4(5) . .
Si1 O15 W6 121.7(7) . .
O12 O15 W6 132.7(9) . .
W5 O15 W6 95.5(5) . .
W4 O15 W6 94.2(5) . .
W6 O16 W4 135.5(9) . .
W4 O17 Cu1 137.7(9) . .
W5 O20 W3 136.9(10) . .
O21B O21A W4 103(4) . .
O21B O21A W1 88(4) . .
W4 O21A W1 150(2) . .
O21A O21B W1 69(4) . .
O21A O21B W4 55(3) . .
W1 O21B W4 118.4(17) . .
W5 O23 W1 135.6(10) 2_556 .
W3 O24 W1 138.6(11) . 2_556
O12 Si1 O12 180.0 2_556 .
O12 Si1 O15 111.2(7) 2_556 .
O12 Si1 O15 68.8(7) . .
O12 Si1 O15 68.8(7) 2_556 2_556
O12 Si1 O15 111.2(7) . 2_556
O15 Si1 O15 180.0 . 2_556
O12 Si1 O8 67.8(8) 2_556 2_556
O12 Si1 O8 112.2(8) . 2_556
O15 Si1 O8 70.7(7) . 2_556
O15 Si1 O8 109.3(7) 2_556 2_556
O12 Si1 O8 112.2(8) 2_556 .
O12 Si1 O8 67.8(8) . .
O15 Si1 O8 109.3(7) . .
O15 Si1 O8 70.7(7) 2_556 .
O8 Si1 O8 180.0(8) 2_556 .
O12 Si1 O3 108.1(7) 2_556 2_556
O12 Si1 O3 71.9(7) . 2_556
O15 Si1 O3 109.1(7) . 2_556
O15 Si1 O3 70.9(7) 2_556 2_556
O8 Si1 O3 73.2(7) 2_556 2_556
O8 Si1 O3 106.8(7) . 2_556
O12 Si1 O3 71.9(7) 2_556 .
O12 Si1 O3 108.1(7) . .
O15 Si1 O3 70.9(7) . .
O15 Si1 O3 109.1(7) 2_556 .
O8 Si1 O3 106.8(7) 2_556 .
O8 Si1 O3 73.2(7) . .
O3 Si1 O3 180.0(9) 2_556 .
N4 Cu1 N4 180.0 . 2_666
N4 Cu1 N6 89.8(7) . .
N4 Cu1 N6 90.2(7) 2_666 .
N4 Cu1 N6 90.2(7) . 2_666
N4 Cu1 N6 89.8(7) 2_666 2_666
N6 Cu1 N6 180.0 . 2_666
N4 Cu1 O17 90.2(6) . 2_666
N4 Cu1 O17 89.8(6) 2_666 2_666
N6 Cu1 O17 95.1(6) . 2_666
N6 Cu1 O17 84.9(6) 2_666 2_666
N4 Cu1 O17 89.8(6) . .
N4 Cu1 O17 90.2(6) 2_666 .
N6 Cu1 O17 84.9(6) . .
N6 Cu1 O17 95.1(6) 2_666 .
O17 Cu1 O17 180.0 2_666 .
N3 Cu2 N11 166.7(7) . 1_455
N3 Cu2 N5 87.1(8) . .
N11 Cu2 N5 90.4(7) 1_455 .
N3 Cu2 N2 89.7(8) . .
N11 Cu2 N2 91.9(7) 1_455 .
N5 Cu2 N2 175.4(8) . .
N3 Cu2 Cl1 102.1(6) . .
N11 Cu2 Cl1 91.1(5) 1_455 .
N5 Cu2 Cl1 94.1(6) . .
N2 Cu2 Cl1 89.7(6) . .
N12 Cu3 N12 180.0 2_767 1_455
N12 Cu3 N1 89.2(8) 2_767 2_667
N12 Cu3 N1 90.8(8) 1_455 2_667
N12 Cu3 N1 90.8(8) 2_767 .
N12 Cu3 N1 89.2(8) 1_455 .
N1 Cu3 N1 180.0 2_667 .
N12 Cu3 Cl1 88.9(6) 2_767 2_667
N12 Cu3 Cl1 91.1(6) 1_455 2_667
N1 Cu3 Cl1 84.5(5) 2_667 2_667
N1 Cu3 Cl1 95.5(5) . 2_667
N12 Cu3 Cl1 91.1(6) 2_767 .
N12 Cu3 Cl1 88.9(6) 1_455 .
N1 Cu3 Cl1 95.5(5) 2_667 .
N1 Cu3 Cl1 84.5(5) . .
Cl1 Cu3 Cl1 180.0(2) 2_667 .
O22 W1 O5 103.6(10) . .
O22 W1 O21A 111.7(13) . .
O5 W1 O21A 87.9(11) . .
O22 W1 O23 101.1(9) . .
O5 W1 O23 85.3(8) . .
O21A W1 O23 147.2(13) . .
O22 W1 O24 103.5(10) . 2_556
O5 W1 O24 152.9(8) . 2_556
O21A W1 O24 80.9(12) . 2_556
O23 W1 O24 90.8(8) . 2_556
O22 W1 O21B 89.5(12) . .
O5 W1 O21B 88.2(10) . .
O21A W1 O21B 22.8(12) . .
O23 W1 O21B 168.6(11) . .
O24 W1 O21B 90.7(11) 2_556 .
O22 W1 O3 154.0(8) . .
O5 W1 O3 59.1(7) . .
O21A W1 O3 52.9(11) . .
O23 W1 O3 96.8(7) . .
O24 W1 O3 94.9(7) 2_556 .
O21B W1 O3 71.9(10) . .
O22 W1 O12 158.6(8) . 2_556
O5 W1 O12 91.2(7) . 2_556
O21A W1 O12 83.8(12) . 2_556
O23 W1 O12 64.4(6) . 2_556
O24 W1 O12 63.1(7) 2_556 2_556
O21B W1 O12 106.5(11) . 2_556
O3 W1 O12 47.4(5) . 2_556
O6 W2 O4A 110.4(13) . .
O6 W2 O5 104.1(9) . .
O4A W2 O5 93.8(12) . .
O6 W2 O7 102.4(9) . .
O4A W2 O7 146.3(13) . .
O5 W2 O7 85.3(8) . .
O6 W2 O9 101.7(10) . .
O4A W2 O9 75.5(13) . .
O5 W2 O9 154.1(8) . .
O7 W2 O9 90.8(8) . .
O6 W2 O4B 88.6(12) . .
O4A W2 O4B 25.5(12) . .
O5 W2 O4B 86.6(11) . .
O7 W2 O4B 167.7(11) . .
O9 W2 O4B 92.5(11) . .
O6 W2 O3 152.8(8) . .
O4A W2 O3 55.0(11) . .
O5 W2 O3 58.9(7) . .
O7 W2 O3 97.4(7) . .
O9 W2 O3 96.4(7) . .
O4B W2 O3 70.4(10) . .
O6 W2 O8 157.7(8) . .
O4A W2 O8 81.9(12) . .
O5 W2 O8 93.1(7) . .
O7 W2 O8 64.5(7) . .
O9 W2 O8 62.4(7) . .
O4B W2 O8 106.8(11) . .
O3 W2 O8 49.4(5) . .
O11 W3 O24 102.8(10) . .
O11 W3 O9 100.9(10) . .
O24 W3 O9 156.2(9) . .
O11 W3 O20 100.5(9) . .
O24 W3 O20 89.4(8) . .
O9 W3 O20 85.0(8) . .
O11 W3 O10 102.5(10) . .
O24 W3 O10 84.9(8) . .
O9 W3 O10 91.3(8) . .
O20 W3 O10 157.0(9) . .
O11 W3 O8 157.1(9) . .
O24 W3 O8 93.6(8) . .
O9 W3 O8 64.1(8) . .
O20 W3 O8 95.4(7) . .
O10 W3 O8 62.9(8) . .
O11 W3 O12 158.3(9) . .
O24 W3 O12 64.6(7) . .
O9 W3 O12 92.3(8) . .
O20 W3 O12 63.4(7) . .
O10 W3 O12 94.2(7) . .
O8 W3 O12 44.5(6) . .
O17 W4 O21A 112.7(13) . .
O17 W4 O4A 111.0(12) . .
O21A W4 O4A 94.4(15) . .
O17 W4 O16 101.3(7) . .
O21A W4 O16 82.2(12) . .
O4A W4 O16 146.0(12) . .
O17 W4 O2 97.8(7) . .
O21A W4 O2 149.2(13) . .
O4A W4 O2 77.4(12) . .
O16 W4 O2 88.3(7) . .
O17 W4 O4B 89.0(11) . .
O21A W4 O4B 91.1(15) . .
O4A W4 O4B 25.8(12) . .
O16 W4 O4B 169.3(11) . .
O2 W4 O4B 93.3(11) . .
O17 W4 O21B 91.7(11) . .
O21A W4 O21B 21.8(12) . .
O4A W4 O21B 96.9(14) . .
O16 W4 O21B 92.2(10) . .
O2 W4 O21B 170.1(11) . .
O4B W4 O21B 84.4(13) . .
O17 W4 O3 155.3(7) . .
O21A W4 O3 54.7(12) . .
O4A W4 O3 55.1(11) . .
O16 W4 O3 97.8(6) . .
O2 W4 O3 98.2(6) . .
O4B W4 O3 71.5(10) . .
O21B W4 O3 71.9(10) . .
O17 W4 O15 156.3(7) . .
O21A W4 O15 85.7(13) . .
O4A W4 O15 81.0(12) . .
O16 W4 O15 65.1(6) . .
O2 W4 O15 63.9(6) . .
O4B W4 O15 106.2(11) . .
O21B W4 O15 107.5(10) . .
O3 W4 O15 48.1(5) . .
O19 W5 O2 98.7(9) . .
O19 W5 O20 101.6(10) . .
O2 W5 O20 88.8(8) . .
O19 W5 O23 100.9(9) . 2_556
O2 W5 O23 160.0(8) . 2_556
O20 W5 O23 90.7(8) . 2_556
O19 W5 O1 99.5(10) . .
O2 W5 O1 88.0(8) . .
O20 W5 O1 158.9(8) . .
O23 W5 O1 85.3(8) 2_556 .
O19 W5 O15 155.8(9) . .
O2 W5 O15 65.3(7) . .
O20 W5 O15 96.3(7) . .
O23 W5 O15 95.0(7) 2_556 .
O1 W5 O15 63.6(7) . .
O19 W5 O12 159.5(9) . .
O2 W5 O12 96.0(7) . .
O20 W5 O12 64.5(7) . .
O23 W5 O12 66.0(7) 2_556 .
O1 W5 O12 95.2(7) . .
O15 W5 O12 44.6(5) . .
O18 W6 O10 102.0(10) . 2_556
O18 W6 O16 100.8(9) . .
O10 W6 O16 84.6(8) 2_556 .
O18 W6 O7 100.4(9) . 2_556
O10 W6 O7 91.0(8) 2_556 2_556
O16 W6 O7 158.7(8) . 2_556
O18 W6 O1 100.3(9) . .
O10 W6 O1 157.6(9) 2_556 .
O16 W6 O1 89.4(8) . .
O7 W6 O1 86.7(8) 2_556 .
O18 W6 O8 156.9(8) . 2_556
O10 W6 O8 62.6(7) 2_556 2_556
O16 W6 O8 95.0(7) . 2_556
O7 W6 O8 64.8(7) 2_556 2_556
O1 W6 O8 96.6(7) . 2_556
O18 W6 O15 156.9(8) . .
O10 W6 O15 95.0(7) 2_556 .
O16 W6 O15 64.9(6) . .
O7 W6 O15 94.9(7) 2_556 .
O1 W6 O15 63.1(7) . .
O8 W6 O15 46.2(5) 2_556 .
C6 N1 N2 103(2) . .
C6 N1 Cu3 132.4(19) . .
N2 N1 Cu3 124.8(14) . .
C1 N2 N1 109(2) . .
C1 N2 Cu2 131.3(19) . .
N1 N2 Cu2 119.7(15) . .
C3 N3 N4 105.5(17) . .
C3 N3 Cu2 127.1(15) . .
N4 N3 Cu2 126.6(13) . .
C2 N4 N3 106.5(15) . .
C2 N4 Cu1 129.8(13) . .
N3 N4 Cu1 123.5(12) . .
C4 N5 N6 106(2) . .
C4 N5 Cu2 127.9(19) . .
N6 N5 Cu2 126.4(14) . .
C5 N6 N5 106.3(19) . .
C5 N6 Cu1 130.0(16) . .
N5 N6 Cu1 122.6(13) . .
C5 N7 C4 104(2) . .
C5 N7 H10 128.1 . .
C4 N7 H10 128.1 . .
C6 N9 C1 103(2) . .
C6 N9 H9 128.3 . .
C1 N9 H9 128.3 . .
C3 N10 C2 104.9(17) . .
C3 N10 Cu4 122.4(15) . .
C2 N10 Cu4 132.5(14) . .
Cu2 Cl1 Cu3 83.4(2) . .
N2 C1 N9 110(3) . .
N2 C1 H1 125.2 . .
N9 C1 H1 125.2 . .
N4 C2 N10 110.7(17) . .
N4 C2 H2 124.6 . .
N10 C2 H2 124.6 . .
N3 C3 N10 112.2(19) . .
N3 C3 H3 123.9 . .
N10 C3 H3 123.9 . .
N5 C4 N7 112(2) . .
N5 C4 H4 124.2 . .
N7 C4 H4 124.2 . .
N7 C5 N6 112(3) . .
N7 C5 H5 123.8 . .
N6 C5 H5 123.8 . .
N1 C6 N9 115(3) . .
N1 C6 H6 122.3 . .
N9 C6 H6 122.3 . .
N8 Cu4 N10 174.2(8) . .
C7 N8 C8 102.3(18) . .
C7 N8 Cu4 128.4(15) . .
C8 N8 Cu4 129.3(16) . .
N11 C7 N8 114(2) . .
N11 C7 H7 123.2 . .
N8 C7 H7 123.2 . .
N12 C8 N8 111(2) . .
N12 C8 H8 124.3 . .
N8 C8 H8 124.3 . .
C7 N11 N12 107.3(18) . .
C7 N11 Cu2 129.4(15) . 1_655
N12 N11 Cu2 122.5(13) . 1_655
C8 N12 N11 105.4(18) . .
C8 N12 Cu3 131.3(16) . 1_655
N11 N12 Cu3 123.2(14) . 1_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 W6 1.901(19) .
O1 W5 1.908(18) .
O2 W5 1.858(18) .
O2 W4 1.957(18) .
O3 Si1 1.697(15) .
O3 W4 2.326(13) .
O3 W1 2.352(14) .
O3 W2 2.357(14) .
O4A O4B 0.88(4) .
O4A W2 1.82(3) .
O4A W4 1.89(3) .
O4B W4 2.01(3) .
O4B W2 2.03(3) .
O5 W1 1.858(19) .
O5 W2 1.865(19) .
O6 W2 1.701(19) .
O7 W2 1.899(18) .
O7 W6 1.899(18) 2_556
O8 Si1 1.642(15) .
O8 O12 1.80(2) .
O8 W3 2.351(15) .
O8 W6 2.396(16) 2_556
O8 W2 2.409(16) .
O9 W3 1.870(19) .
O9 W2 1.90(2) .
O10 W6 1.87(2) 2_556
O10 W3 1.932(19) .
O11 W3 1.654(19) .
O12 Si1 1.587(15) .
O12 O15 1.81(2) .
O12 W5 2.389(14) .
O12 W3 2.411(15) .
O12 W1 2.447(17) 2_556
O15 Si1 1.620(14) .
O15 W5 2.383(14) .
O15 W4 2.392(15) .
O15 W6 2.411(14) .
O16 W6 1.889(17) .
O16 W4 1.913(17) .
O17 W4 1.693(16) .
O17 Cu1 2.406(16) .
O18 W6 1.689(16) .
O19 W5 1.652(19) .
O20 W5 1.871(19) .
O20 W3 1.925(18) .
O21A O21B 0.79(4) .
O21A W4 1.74(3) .
O21A W1 1.91(3) .
O21B W1 2.03(3) .
O21B W4 2.06(3) .
O22 W1 1.658(19) .
O23 W5 1.885(17) 2_556
O23 W1 1.910(17) .
O24 W3 1.850(19) .
O24 W1 1.91(2) 2_556
Si1 O12 1.587(15) 2_556
Si1 O15 1.620(14) 2_556
Si1 O8 1.642(15) 2_556
Si1 O3 1.697(15) 2_556
Cu1 N4 1.980(16) .
Cu1 N4 1.980(16) 2_666
Cu1 N6 2.007(17) .
Cu1 N6 2.007(17) 2_666
Cu1 O17 2.406(16) 2_666
Cu2 N3 1.936(19) .
Cu2 N11 1.975(17) 1_455
Cu2 N5 2.009(19) .
Cu2 N2 2.05(2) .
Cu2 Cl1 2.543(7) .
Cu3 N12 1.982(19) 2_767
Cu3 N12 1.982(19) 1_455
Cu3 N1 2.012(18) 2_667
Cu3 N1 2.012(18) .
Cu3 Cl1 2.769(7) 2_667
Cu3 Cl1 2.769(7) .
W1 O24 1.91(2) 2_556
W1 O12 2.447(17) 2_556
W5 O23 1.885(17) 2_556
W6 O10 1.87(2) 2_556
W6 O7 1.899(18) 2_556
W6 O8 2.396(16) 2_556
N1 C6 1.28(3) .
N1 N2 1.37(2) .
N2 C1 1.28(3) .
N3 C3 1.32(3) .
N3 N4 1.40(2) .
N4 C2 1.34(3) .
N5 C4 1.30(3) .
N5 N6 1.37(2) .
N6 C5 1.33(3) .
N7 C5 1.29(3) .
N7 C4 1.37(4) .
N7 H10 0.8600 .
N9 C6 1.29(4) .
N9 C1 1.34(4) .
N9 H9 0.8600 .
N10 C3 1.35(3) .
N10 C2 1.35(3) .
N10 Cu4 1.880(16) .
C1 H1 0.9300 .
C2 H2 0.9300 .
C3 H3 0.9300 .
C4 H4 0.9300 .
C5 H5 0.9300 .
C6 H6 0.9300 .
Cu4 N8 1.861(17) .
N8 C7 1.33(3) .
N8 C8 1.37(3) .
C7 N11 1.27(3) .
C7 H7 0.9300 .
C8 N12 1.31(3) .
C8 H8 0.9300 .
N11 N12 1.38(2) .
N11 Cu2 1.975(17) 1_655
N12 Cu3 1.982(18) 1_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
W2 O4A O4B W4 -142.4(18) . .
W4 O4A O4B W2 142.4(18) . .
W3 O8 O12 Si1 179.3(7) . .
W6 O8 O12 Si1 101.2(12) 2_556 .
W2 O8 O12 Si1 -100.7(11) . .
Si1 O8 O12 O15 44.7(7) . .
W3 O8 O12 O15 -136.0(8) . .
W6 O8 O12 O15 145.9(11) 2_556 .
W2 O8 O12 O15 -56.0(12) . .
Si1 O8 O12 W5 108.0(12) . .
W3 O8 O12 W5 -72.7(11) . .
W6 O8 O12 W5 -150.8(9) 2_556 .
W2 O8 O12 W5 7.4(19) . .
Si1 O8 O12 W3 -179.3(7) . .
W6 O8 O12 W3 -78.1(11) 2_556 .
W2 O8 O12 W3 80.0(9) . .
Si1 O8 O12 W1 -105.4(10) . 2_556
W3 O8 O12 W1 73.9(9) . 2_556
W6 O8 O12 W1 -4.1(18) 2_556 2_556
W2 O8 O12 W1 154.0(7) . 2_556
O8 O12 O15 Si1 -45.4(7) . .
W5 O12 O15 Si1 179.2(7) . .
W3 O12 O15 Si1 -106.5(12) . .
W1 O12 O15 Si1 104.2(10) 2_556 .
Si1 O12 O15 W5 -179.2(7) . .
O8 O12 O15 W5 135.4(8) . .
W3 O12 O15 W5 74.3(10) . .
W1 O12 O15 W5 -75.1(9) 2_556 .
Si1 O12 O15 W4 102.8(10) . .
O8 O12 O15 W4 57.4(12) . .
W5 O12 O15 W4 -78.0(9) . .
W3 O12 O15 W4 -3.7(18) . .
W1 O12 O15 W4 -153.0(7) 2_556 .
Si1 O12 O15 W6 -102.9(11) . .
O8 O12 O15 W6 -148.2(10) . .
W5 O12 O15 W6 76.4(9) . .
W3 O12 O15 W6 150.6(8) . .
W1 O12 O15 W6 1.3(17) 2_556 .
W4 O21A O21B W1 -152(3) . .
W1 O21A O21B W4 152(3) . .
O8 O12 Si1 O15 122.8(9) . .
W5 O12 Si1 O15 -0.9(8) . .
W3 O12 Si1 O15 123.5(11) . .
W1 O12 Si1 O15 -119.1(10) 2_556 .
O8 O12 Si1 O15 -57.2(9) . 2_556
O15 O12 Si1 O15 180.000(4) . 2_556
W5 O12 Si1 O15 179.1(8) . 2_556
W3 O12 Si1 O15 -56.5(11) . 2_556
W1 O12 Si1 O15 60.9(10) 2_556 2_556
O8 O12 Si1 O8 180.001(6) . 2_556
O15 O12 Si1 O8 57.2(9) . 2_556
W5 O12 Si1 O8 56.4(12) . 2_556
W3 O12 Si1 O8 -179.2(8) . 2_556
W1 O12 Si1 O8 -61.9(10) 2_556 2_556
O15 O12 Si1 O8 -122.8(9) . .
W5 O12 Si1 O8 -123.6(12) . .
W3 O12 Si1 O8 0.8(8) . .
W1 O12 Si1 O8 118.1(10) 2_556 .
O8 O12 Si1 O3 -117.4(9) . 2_556
O15 O12 Si1 O3 119.8(8) . 2_556
W5 O12 Si1 O3 118.9(11) . 2_556
W3 O12 Si1 O3 -116.7(10) . 2_556
W1 O12 Si1 O3 0.7(7) 2_556 2_556
O8 O12 Si1 O3 62.6(9) . .
O15 O12 Si1 O3 -60.2(8) . .
W5 O12 Si1 O3 -61.1(11) . .
W3 O12 Si1 O3 63.3(10) . .
W1 O12 Si1 O3 -179.3(7) 2_556 .
O12 O15 Si1 O12 179.999(3) . 2_556
W5 O15 Si1 O12 -179.2(8) . 2_556
W4 O15 Si1 O12 60.4(10) . 2_556
W6 O15 Si1 O12 -57.3(11) . 2_556
W5 O15 Si1 O12 0.8(8) . .
W4 O15 Si1 O12 -119.6(10) . .
W6 O15 Si1 O12 122.7(11) . .
O12 O15 Si1 O8 -124.4(9) . 2_556
W5 O15 Si1 O8 -123.5(11) . 2_556
W4 O15 Si1 O8 116.0(10) . 2_556
W6 O15 Si1 O8 -1.7(8) . 2_556
O12 O15 Si1 O8 55.6(9) . .
W5 O15 Si1 O8 56.5(11) . .
W4 O15 Si1 O8 -64.0(10) . .
W6 O15 Si1 O8 178.3(8) . .
O12 O15 Si1 O3 -60.9(8) . 2_556
W5 O15 Si1 O3 -60.0(10) . 2_556
W4 O15 Si1 O3 179.6(7) . 2_556
W6 O15 Si1 O3 61.8(10) . 2_556
O12 O15 Si1 O3 119.1(8) . .
W5 O15 Si1 O3 120.0(10) . .
W4 O15 Si1 O3 -0.4(7) . .
W6 O15 Si1 O3 -118.2(10) . .
O12 O8 Si1 O12 180.000(7) . 2_556
W3 O8 Si1 O12 179.2(8) . 2_556
W6 O8 Si1 O12 54.5(12) 2_556 2_556
W2 O8 Si1 O12 -61.1(11) . 2_556
W3 O8 Si1 O12 -0.8(8) . .
W6 O8 Si1 O12 -125.5(12) 2_556 .
W2 O8 Si1 O12 118.9(11) . .
O12 O8 Si1 O15 -56.2(9) . .
W3 O8 Si1 O15 -57.0(11) . .
W6 O8 Si1 O15 178.3(8) 2_556 .
W2 O8 Si1 O15 62.7(10) . .
O12 O8 Si1 O15 123.8(9) . 2_556
W3 O8 Si1 O15 123.0(11) . 2_556
W6 O8 Si1 O15 -1.7(8) 2_556 2_556
W2 O8 Si1 O15 -117.3(10) . 2_556
O12 O8 Si1 O3 61.8(8) . 2_556
W3 O8 Si1 O3 61.0(10) . 2_556
W6 O8 Si1 O3 -63.7(10) 2_556 2_556
W2 O8 Si1 O3 -179.4(7) . 2_556
O12 O8 Si1 O3 -118.2(8) . .
W3 O8 Si1 O3 -119.0(10) . .
W6 O8 Si1 O3 116.3(10) 2_556 .
W2 O8 Si1 O3 0.6(7) . .
W4 O3 Si1 O12 -120.6(9) . 2_556
W1 O3 Si1 O12 0.7(8) . 2_556
W2 O3 Si1 O12 120.2(9) . 2_556
W4 O3 Si1 O12 59.4(9) . .
W1 O3 Si1 O12 -179.3(8) . .
W2 O3 Si1 O12 -59.8(9) . .
W4 O3 Si1 O15 0.4(7) . .
W1 O3 Si1 O15 121.7(9) . .
W2 O3 Si1 O15 -118.7(9) . .
W4 O3 Si1 O15 -179.6(7) . 2_556
W1 O3 Si1 O15 -58.3(9) . 2_556
W2 O3 Si1 O15 61.3(9) . 2_556
W4 O3 Si1 O8 -61.5(9) . 2_556
W1 O3 Si1 O8 59.8(9) . 2_556
W2 O3 Si1 O8 179.4(7) . 2_556
W4 O3 Si1 O8 118.5(9) . .
W1 O3 Si1 O8 -120.2(9) . .
W2 O3 Si1 O8 -0.6(7) . .
W2 O5 W1 O22 -149.4(17) . .
W2 O5 W1 O21A -38(2) . .
W2 O5 W1 O23 110.3(18) . .
W2 O5 W1 O24 28(3) . 2_556
W2 O5 W1 O21B -60.4(19) . .
W2 O5 W1 O3 9.5(14) . .
W2 O5 W1 O12 46.1(17) . 2_556
O4B O4A W2 O6 -33(4) . .
W4 O4A W2 O6 -116(3) . .
O4B O4A W2 O5 74(3) . .
W4 O4A W2 O5 -9(3) . .
O4B O4A W2 O7 161(3) . .
W4 O4A W2 O7 78(4) . .
O4B O4A W2 O9 -130(4) . .
W4 O4A W2 O9 147(4) . .
W4 O4A W2 O4B -83(5) . .
O4B O4A W2 O3 121(4) . .
W4 O4A W2 O3 38(3) . .
O4B O4A W2 O8 167(4) . .
W4 O4A W2 O8 84(3) . .
W1 O5 W2 O6 147.3(17) . .
W1 O5 W2 O4A 35(2) . .
W1 O5 W2 O7 -111.1(18) . .
W1 O5 W2 O9 -29(3) . .
W1 O5 W2 O4B 59.7(19) . .
W1 O5 W2 O3 -9.5(14) . .
W1 O5 W2 O8 -47.0(17) . .
W6 O7 W2 O6 -154.5(16) 2_556 .
W6 O7 W2 O4A 12(3) 2_556 .
W6 O7 W2 O5 102.0(17) 2_556 .
W6 O7 W2 O9 -52.4(17) 2_556 .
W6 O7 W2 O4B 53(6) 2_556 .
W6 O7 W2 O3 44.2(17) 2_556 .
W6 O7 W2 O8 6.3(13) 2_556 .
W1 O24 W3 O11 -151.5(16) 2_556 .
W1 O24 W3 O9 25(3) 2_556 .
W1 O24 W3 O20 -50.8(16) 2_556 .
W1 O24 W3 O10 106.9(17) 2_556 .
W1 O24 W3 O8 44.5(16) 2_556 .
W1 O24 W3 O12 9.7(13) 2_556 .
W2 O9 W3 O11 -152.0(16) . .
W2 O9 W3 O24 31(3) . .
W2 O9 W3 O20 108.3(16) . .
W2 O9 W3 O10 -49.0(17) . .
W2 O9 W3 O8 9.8(13) . .
W2 O9 W3 O12 45.3(16) . .
Cu1 O17 W4 O21A 174.4(15) . .
Cu1 O17 W4 O4A 70.0(17) . .
Cu1 O17 W4 O16 -99.3(13) . .
Cu1 O17 W4 O2 -9.6(14) . .
Cu1 O17 W4 O4B 83.7(15) . .
Cu1 O17 W4 O21B 168.0(15) . .
Cu1 O17 W4 O3 120.6(14) . .
Cu1 O17 W4 O15 -47(2) . .
O21B O21A W4 O17 -17(4) . .
W1 O21A W4 O17 -126(4) . .
O21B O21A W4 O4A 98(4) . .
W1 O21A W4 O4A -11(5) . .
O21B O21A W4 O16 -116(4) . .
W1 O21A W4 O16 135(4) . .
O21B O21A W4 O2 170(3) . .
W1 O21A W4 O2 61(6) . .
O21B O21A W4 O4B 72(4) . .
W1 O21A W4 O4B -37(4) . .
W1 O21A W4 O21B -109(6) . .
O21B O21A W4 O3 138(4) . .
W1 O21A W4 O3 29(4) . .
O21B O21A W4 O15 178(4) . .
W1 O21A W4 O15 69(4) . .
O4B O4A W4 O17 33(4) . .
W2 O4A W4 O17 118(3) . .
O4B O4A W4 O21A -83(3) . .
W2 O4A W4 O21A 2(4) . .
O4B O4A W4 O16 -166(3) . .
W2 O4A W4 O16 -81(4) . .
O4B O4A W4 O2 127(3) . .
W2 O4A W4 O2 -148(4) . .
W2 O4A W4 O4B 85(5) . .
O4B O4A W4 O21B -61(3) . .
W2 O4A W4 O21B 23(4) . .
O4B O4A W4 O3 -124(4) . .
W2 O4A W4 O3 -39(3) . .
O4B O4A W4 O15 -168(3) . .
W2 O4A W4 O15 -83(3) . .
W4 O2 W5 O19 157.6(15) . .
W4 O2 W5 O20 -100.9(14) . .
W4 O2 W5 O23 -12(3) . 2_556
W4 O2 W5 O1 58.3(14) . .
W4 O2 W5 O15 -3.4(11) . .
W4 O2 W5 O12 -36.7(14) . .
W3 O20 W5 O19 -155.7(15) . .
W3 O20 W5 O2 105.7(15) . .
W3 O20 W5 O23 -54.4(15) . 2_556
W3 O20 W5 O1 24(3) . .
W3 O20 W5 O15 40.7(15) . .
W3 O20 W5 O12 8.5(12) . .
W4 O16 W6 O18 -155.0(14) . .
W4 O16 W6 O10 103.8(15) . 2_556
W4 O16 W6 O7 25(3) . 2_556
W4 O16 W6 O1 -54.6(14) . .
W4 O16 W6 O8 41.9(14) . 2_556
W4 O16 W6 O15 5.7(11) . .
C6 N1 N2 C1 -3(3) . .
Cu3 N1 N2 C1 179(2) . .
C6 N1 N2 Cu2 -178.8(18) . .
Cu3 N1 N2 Cu2 4(2) . .
C3 N3 N4 C2 4(2) . .
Cu2 N3 N4 C2 173.4(16) . .
C3 N3 N4 Cu1 -171.3(15) . .
Cu2 N3 N4 Cu1 -2(2) . .
C4 N5 N6 C5 4(3) . .
Cu2 N5 N6 C5 -178.1(15) . .
C4 N5 N6 Cu1 173.3(17) . .
Cu2 N5 N6 Cu1 -9(2) . .
N1 N2 C1 N9 2(3) . .
Cu2 N2 C1 N9 177.5(17) . .
C6 N9 C1 N2 -1(3) . .
N3 N4 C2 N10 -2(2) . .
Cu1 N4 C2 N10 172.6(14) . .
C3 N10 C2 N4 0(2) . .
Cu4 N10 C2 N4 -174.8(15) . .
N4 N3 C3 N10 -4(3) . .
Cu2 N3 C3 N10 -173.9(15) . .
C2 N10 C3 N3 3(3) . .
Cu4 N10 C3 N3 178.1(15) . .
N6 N5 C4 N7 -6(3) . .
Cu2 N5 C4 N7 176.0(17) . .
C5 N7 C4 N5 6(3) . .
C4 N7 C5 N6 -3(3) . .
N5 N6 C5 N7 0(3) . .
Cu1 N6 C5 N7 -168.6(16) . .
N2 N1 C6 N9 3(3) . .
Cu3 N1 C6 N9 179.9(18) . .
C1 N9 C6 N1 -1(4) . .
C8 N8 C7 N11 0(3) . .
Cu4 N8 C7 N11 -178.8(17) . .
C7 N8 C8 N12 0(3) . .
Cu4 N8 C8 N12 179.0(18) . .
N8 C7 N11 N12 0(3) . .
N8 C7 N11 Cu2 169.4(16) . 1_655
N8 C8 N12 N11 0(3) . .
N8 C8 N12 Cu3 178.4(18) . 1_655
C7 N11 N12 C8 0(3) . .
Cu2 N11 N12 C8 -170.3(16) 1_655 .
C7 N11 N12 Cu3 -178.3(17) . 1_655
Cu2 N11 N12 Cu3 11(3) 1_655 1_655
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.000 0.000 340 156 ' '
